Orientational order-disorder γ ↔ β ↔ α′ ↔ α phase transitions in Sr2B2O5 pyroborate and crystal structures of β and α phases
Volkov, Sergey; Dušek, Michal; Bubnova, Rimma; Krzhizhanovskaya, Maria; Ugolkov, Valery; Obozova, Ekaterina; Filatov, Stanislav; Acta Crystallographica Section B Structural Science, Crystal Engineering and Materials 73 (2017) 1056–; doi:10.1107/S2052520617012689

data_2021892
_publ_section_title
;
 Orientational order-disorder \g &#x2194; \b &#x2194; \a&#x2032; &#x2194;
 \a phase transitions in Sr2B2O5 pyroborate and crystal structures of \b
 and \a phases
;
_journal_coeditor_code           DQ5023
_journal_issue                   6
_journal_name_full
'Acta Crystallographica Section B Structural Science, Crystal Engineering and Materials'
_journal_page_first              1056
_journal_paper_doi               10.1107/S2052520617012689
_journal_volume                  73
_journal_year                    2017
_chemical_formula_sum            'B2 O5 Sr2'
_chemical_formula_weight         276.9
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_space_group_ssg_name            P-1(\a\b\g)0
_symmetry_cell_setting           triclinic
_cell_angle_alpha                89.994(11)
_cell_angle_beta                 92.008(11)
_cell_angle_gamma                90.038(11)
_cell_formula_units_Z            2
_cell_length_a                   3.9001(11)
_cell_length_b                   5.3685(7)
_cell_length_c                   11.8671(16)
_cell_measurement_reflns_used    2199
_cell_measurement_temperature    583
_cell_measurement_theta_max      27.62
_cell_measurement_theta_min      4.15
_cell_modulation_dimension       1
_cell_volume                     248.32(8)
_computing_cell_refinement       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_diffrn_ambient_temperature      295
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 5.1783
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.95
_diffrn_measurement_device_type  'Xcalibur, AtlasS2, Gemini ultra'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0618
_diffrn_reflns_av_unetI/netI     0.0609
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_index_m_1_max 3
_diffrn_reflns_limit_index_m_1_min -3
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            42872
_diffrn_reflns_theta_full        27.58
_diffrn_reflns_theta_max         27.97
_diffrn_reflns_theta_min         3.44
_diffrn_source                   'fine-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    21.549
_exptl_absorpt_correction_T_max  0.186
_exptl_absorpt_correction_T_min  0.037
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.41 (Rigaku Oxford Diffraction, 2015)
Analytical numeric absorption correction using a multifaceted crystal
   model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    3.7028
_exptl_crystal_F_000             252
_exptl_crystal_size_max          0.269
_exptl_crystal_size_mid          0.145
_exptl_crystal_size_min          0.105
_refine_diff_density_max         1.15
_refine_diff_density_min         -1.12
_refine_ls_extinction_coef       790(30)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.26
_refine_ls_goodness_of_fit_ref   1.15
_refine_ls_number_constraints    0
_refine_ls_number_parameters     366
_refine_ls_number_reflns         11221
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1317
_refine_ls_R_factor_gt           0.0412
_refine_ls_shift/su_max          0.0140
_refine_ls_shift/su_mean         0.0006
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0423
_refine_ls_wR_factor_ref         0.0601
_reflns_number_gt                4809
_reflns_number_total             11221
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            dq5023sup1.cif
_cod_data_source_block           Iv
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/IUCr/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_database_code               2021892
_jana_cell_commen_supercell_matrix_1_1 2
_jana_cell_commen_supercell_matrix_1_2 -2
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 1
_jana_cell_commen_supercell_matrix_2_2 2
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0